Informatics for Chemical Crystallography

 Amie Heath
 5 months ago
 Views:
Transcription
1 Materials Informatics Overview Informatics for Chemical Crystallography Changwon Suh and Krishna Rajan A fundamental question in inorganic crystallography is the relationship between chemical stoichiometry and crystal structure. The relationship between specifi c compounds and specifi c crystal structures is usually developed heuristically by surveying crystallographic data of known compounds. This process of structure chemistry association has laid the historical foundation for identifying crystal structure prototypes and structural classifi cations. This paper demonstrates how informatics can quantitatively accelerate the discovery of structure chemistry relationships but also be used as the foundation for developing structure chemistry property relationships. INTRODUCTION The search for stable compound structures based on information about the constituent elements is a classic crystal chemistry problem. When predicting new possible materials traditionally structure maps have been used to search for stable phases. Structure mapping has played an important role as an a priori guide for finding stable phases 1 and serving as a visualization tool for structure property relationships in a bivariate way. Physical factors governing stable crystal structures serve as the coordinates of structure maps. After physical factors are carefully chosen each compound can be spatially identified by its structure type. From the viewpoint of informatics a structure map is a classification tool whereby through the choice of appropriate coordinates one can map clustering of crystalstructurerelated data. There is of course a long and distinguished tradition of such maps including Mooser Pearson plots 2 Philips and van Vechten diagrams 34 Goldschmidt diagrams 5 and Pettifor plots 16 just to mention a few examples. Each of these mapping schemes identifies some key parameters related to electronic or crystal structure information which are placed on orthogonal axes and the occurrence of a given crystal chemistry is then plotted accordingly. The resulting diagram maps out the relative position of structure types from which one tries to discern qualitatively if there are strong associations of certain crystal types to certain bivariate combinations of parameters. This however does not address the multivariate nature of the parameters associated with crystal chemistry and hence provides a strong motivation to apply data dimensionality reduction techniques. STRUCTURE CHEMISTRY CLASSIFICATION How would you describe the overall significance of this paper? Informatics can provide an accelerated and robust means of discovering structurechemistryproperty relationships. describe this work to a materials science and engineering professional with no experience in your technical specialty? This paper shows how informatics can be used as a new computational tool to aid in materials discovery and design. describe this work to a layperson? A new computational approach is proposed for discovering what parameters govern which crystal structures are formed for different chemical compounds. C. Suh and K. Rajan 7 have demonstrated a strategy for developing structure maps without any a priori assumption of which two parameters are to be selected for developing a structure map. This is treated as a multivariate analysis problem where we collectively input many of the wellknown and accepted variables that can have an influence (termed latent variables in the jargon of informatics) on the occurrence of a given type of crystal structure. This approach can be used to identify the appropriate selection of variables for use in twodimensional structure maps. The first step in this process is applying data dimensionality reduction techniques such as principle component analysis (PCA). The computational details are not described here but the reader is referred to numerous standard texts in the field 89 as well as papers that have used this specific multivariate data analysis method in materials science applications The generated data set includes crystallographic parameters informaticsbased prediction of bulk moduli electronic bonding and combined parameters and therefore it contains large amounts of factors governing crystal structure (Table I). The PCA loading map separates structural governing factors based on their correlations and relative impacts on PCA models. Through the process of eigenvector decomposition in PCA the original data is decomposed by two matrices: loadings and scores. The loadings are the weights for each original variable while the scores are the projection of the sample on a rotated coordinate system. Thus PCA loading plots map the correlation between physical parameters and score plots map the correlation between spinel nitrides. Interpretations of the loading plot are twofold: 48 JOM January 2009
2 Degree of correlation between variables: angle between variableoriginvariable where the origin is (00) position. Relative impact of variables on PCA model: distance from the origin to variable. The degree of correlation between variables is determined by the angles (cosine) between them. If the angle between two variables at the origin is then = 0 for highly positively correlated variables = 180 for highly inversely correlated variables and = 90 if no correlation exists. Therefore a PCA loading plot captures all the possible correlations within a multivariate data set in twodimensional spaces. Since PCA reduces the dimensionality of variables with a minimal loss of information it should be noted that correlations on a PCA map depend on the variance captured by the confined dimensions. This means they could be different from the bivariate correlation coefficient (e.g. Pearson s). On the other hand the relative impact of each variable can be identified by measuring the distance from the origin. Interpretation of the score plot is the same as the loading plot. The loading plot of PCA separates multiple descriptors by their characteristics helps to detect key descriptors and shows bond characteristics in terms of structural and electronic bonding parameters. Overall the reason to form the shape of the shell for grouped properties is their similar impacts on the PCA model. For instance all the parameters related with cell dimensions have similar effects on the two LV PCA models. The degree of impact on the PCA model is based on cell dimension parameters and the degree of bond strength from the radius of each shell. Thus one may rank the relative degree of impact as: electronegativity difference bond length and polyhedral volume > pseudopotential radii > bulk modulus > effective charge > bond order. Using AB 2 N 4 spinel nitrides as a template Suh and Rajan have assessed the statistical interdependency of each of the descriptors that may influence chemistry structure property relationships. Using PCA they demonstrated that classical versions of structure maps (from the early work of Hill 20 ) based on heuristic observations for this class of crystal chemistry can in fact be reproduced via data mining. The informatics approach also provides an alternative method for visualizing structure maps Origin of Descriptors Table I. Governing Factors for Spinel Nitrides AB 2 N 4 * Descriptors Abinitio derived parameters a (lattice constant) 2. u (anion parameter) 3. BL AN =A 8a 4. BL BN =B 16d 5. Q * (effective charge) A 6. Q * B 7. Q * N 8. BO (bond order of crystal) Cry 9. BO AN 10. BO BN A Pseudopotential orbital radii 11. r related parameters B 12. r AN 13. R BN 14. R AN 15. R 16. BN R as well as interpreting structureproperty relationships. Apart from being able to reproduce earlier versions of structure maps an example is also developed for the case of a new informaticsbased structure map for spinel ni 17. R 18. R 19. PR (weighted differences of Zunger s pseudopotential radii sums) Crystallographic parameters 20. A 8a  16c or B 16d  8b48f (bond lengths and polyhedral 21. A 8a  48f volumes) from a and u 22. A 8a  2nd n.n. B B or B  48f 16d 16d 16d 16c 23. A 8a B 16d B 16d  8b or B 16d  2nd n.n. 48f 24. A 8a A 8a or A 8a  8b 25. (N 32e ) (N 32e ) (N 32e ) b 29. ( 48f ) ( 48f ) c 32. BL AN /BL BN 33. V (A8a) tet 34. V (A8b) tet 35. V (A48f) tet 36. V (B16d) oct 37. V (B16e) oct 38. V (N32e) oct Interbond angles from 39. ANA spinel structure 40. NBN 41. BNB 42. ANB *. NAN (constant= ) Derived parameters 43. Q * N Q* B (combinations of parameters 44. Q * N Q* A or miscellaneous) EN (from electronegativity of elements) 46. B 0 (from prediction of Partial Least Squares) Note that expressions of variables for bond lengths and polyhedral volumes follows the work of Sickafus et al. 10 A and B represent tetrahedral (tet) and octahedral (oct) cation sites respectively and and represent an octahedral and tetrahedral vacancy respectively. * It is not used for PCA model because it is a constant. Vol. 61 No. 1 JOM 49
3 a Figure 1. (a) Hill s map for spinel nitrides: Anion parameter (u) gives the ratio of the octahedral to tetrahedral bond lengths and octahedral bond length is the same as tetrahedral bond length when u= (b) PCA score map of site occupancy based on complex interactions between bonding and crystal chemistry (governing factors in Table I). Using PCA it is demonstrated that Hill s map based on heuristic observations for this class of crystal chemistry in fact is reproduced via data mining techniques since the shape of this map is similar to Hill s map for spinel nitrides. For clarity some spinel nitrides are labeled. b trides showing data clustering associated with site occupancy. Structure maps are essentially classification maps. They show how crystal chemistry and the associated structure can be clustered according to the pair of parameters that define the axes of the plot. As noted at the beginning of this paper historically there are numerous such maps that have been proposed based on different sets of parameters that reflect bonding and structure. 14 It is instructive to compare the multivariate PCA score plot (Figure 1) which contains all 46 variables simultaneously with the structure map proposed by Hill (Figure 1a 20 ) which used just the anion parameter and lattice constant of the spinel oxides and sulfides. This striking similarity serves to highlight that the principal components (i.e. principal contributions) are primarily capturing lattice constants and anion parameters which were identified as the most important parameters in PC1 and PC2 respectively in the loading plot. While the PCA score map effectively serves as a high dimensional structure map Hill s structure map serves as a validation of the datamining analysis. QSARs FOR STRUCTURE PROPERTY RELATIONSHIPS While a fundamental tenet in materials science is to establish structureproperty relationships it is the life sciences and organic chemistry community that has formally introduced the concept of quantitative structure activity (or also termed property) relationships (QSAR or QSPR). Unlike classical materialsscience approaches which relate structure and function Figure 2. The original Hill map which was derived for spinel oxides and sulfides. The new data for spinel nitrides are added for comparison. The spinel nitrides and oxides are clustered approximately in the same region of the Hill structure map; however the range of lattice constants observed for oxides for the same variability in anion parameter is narrower than it is for the nitride. Note that each equiline of bond length is drawn for visually clear separation of oxides sulfides and nitrides by setting limiting values of bond length. Note that black lines of equibond length in the figure were calculated from geometric relations of interatomic distances as a function of a and u in a spinel structure (i.e. BL 3a(u 1/ 4) A N and BL a[2(u 3 / 8) (5 / 8 u) ]. B N through physically based models (e.g. grain size and strength through the Hall Petch relationship) QSARs are derived from a model independent approach; sometimes referred to as soft modeling. The orthogonality of the principal 50 JOM January 2009
4 components eliminates the multidimensional problem but the problem of choosing an optimum subset of predictors remains. A possible strategy is to keep only a few of the first components; however they are chosen to explain X rather than Y and so nothing guarantees that the principal components which explain X are relevant for Y. The next step in examining the data in PCA space is to see if we can develop models based on this new data set. In other words we want to try to set up a regression model between the scores and not just the original data. Partial least squares (PLS) regression models are based on principal components of both the independent data X and the dependent data Y. The central idea is to calculate the principal component scores of the X and the Y data matrix and to set up a regression model between the scores (and not the original data). Hence in contrast to PCA PLS regression finds components from X that are also relevant for Y. Specifically PLS regression searches for a set of components (called latent vectors) that performs a simultaneous decomposition of X and Y with the constraint that these components explain as much as possible of the covariance between X and Y. This step generalizes PCA. It is followed by a regression step where the decomposition of X is used to predict Y. As noted by R.D. Tobias 21 the emphasis in PLS is on predicting the responses and not necessarily on trying to understand the underlying relationship between the variables. For example PLS is not usually appropriate for screening out factors that have a negligible effect on the response. However when prediction is the goal and there is no practical need to limit the number of measured factors PLS can be a useful tool. When the number of factors gets too large (for example greater than the number of observations) you are likely to get a model that fits the sampled data perfectly but that will fail to predict new data well. This phenomenon is called overfitting. In such cases although there are many manifest factors there may be only a few underlying or latent factors that account for most of the variation in the response. The general idea of PLS is to try to extract these latent factors accounting for as much of the manifest factor variation as possible while modeling the responses well. For this reason the acronym PLS has also been taken to mean projection to latent structure. Hence PLS expresses a dependent variable (target property) in terms of linear combinations of the principal components. While the descriptors themselves may be interdependent (covariant) the PCs so generated are independent (orthogonal). The PLS equation assumes the following form for the case of n descriptors to find the correlation factors between X and Y that have maximum variance: 22 Target property = a o + a 1 (PC 1 ) + a 2 (PC 2 ) + a 3 (PC 3 ) + a n (PC n ) (1) The multidimensional space of X is reduced to the Adimensional hyper plane. Since the scores are good predictors of Y the correlation of Y is formed on this hyper plane. As in PCA the loadings of X represent the orientation of each of the components of the hyper plane. The PLS method can be applied to rationalize the materials attributes relevant to materials function or property and this permits one to use PLS methods to develop explicit quantitative relationships that identify the relative contributions of different data descriptors and the resulting relationship between all these descriptors as a linear combination to the final property. For instance Suh and Rajan explored the attributes used in electronic structure calculations and their influence on predicting bulk modulus. 19 Using PLS a QSAR was developed relating bulk modulus of AB 2 N 4 spinels with a variety of Bulk modulus = EN u BL A N BL B N Q* tet Q* oct Q* N (2) where EN = weighted electronegativity difference; u = internal anion parameter; BL A N = A N bond length; BL B N = BN bond length; Q* tet = Mulliken effective charge for tetrahedral site ion; Q* oct = Mulliken effective charge for octahedral site ion; and Q* N = Mulliken effective charge for N ion. By systematically exploring the number and type of variables needed they found very strong agreement in being able to predict properties consistent with abinitio calculations based strictly on a datadriven analysis. Based on our QSAR formulation the role of the effective charge (Q*) in enhancing modulus is particularly notable. This is consistent with theoretical studies 1123 that show it is the effective charge parameter which helps to define the degree of charge transfer and the level of covalency associated with the specific site occupancy of a given species. Abinitio calculations of this effective Figure 3. An example of a data table and quantum mechanical descriptors used in PLSbased predictions of bulk modulus as compared to abinitio calculations. 19 Vol. 61 No. 1 JOM 51
5 charge can then be used as a major screening parameter in identifying promising crystal chemistries for promoting the modulus. Hence using PLS to develop a QSAR formulation combined with an interpretation of the physics governing these materials can indeed be valuable. Our predictions fit well with systems of similar electronic structure and allow us to clearly identify outliers based on these quantum mechanical calculations. Based on these predictions we can now seriously and effectively accelerate materials design by focusing on promising candidate chemistries. Those selected can then be subjected to further analysis via experimentation and computational methods to validate crystalstructurelevel properties. The data generated by these selective experiments and computations also serve to refine the next generation of training data for another iterative round of data mining which permits a further refinement of highthroughput predictions. See the sidebar for details on analytical expressions for crystal chemistry. ACKNOWLEDGEMENT We gratefully acknowledge support from the National Science Foundation International Materials Institute Program for Combinatorial Sciences and Materials Informatics Collaboratory (CoSMICIMI) Grant no. DMR ; Air Force Office of Scientific Research Grant no. FA and no. FA and the Defense Advanced Research Programs Agency Center for Interfacial Engineering for MEMS (CIEMS) Grant no B. References 1. D.G. Pettifor Structure Mapping Intermetallic Compounds: Principles and Practice ed. J.H. Westbrook and R.L. Fleischer Vol. 1 (Chichester U.K.: John Wiley & Sons 1995) pp E. Mooser and W.B. Pearson On the Crystal Chemistry of Normal Valence Compounds Acta Cryst. 12 (1959) pp W. Andreoni et al. Hardcore Pseudopotentials and Structural Maps of Solids Phys. Rev. B 20 (12) (1979) p J.C. Phillips and J.A. Van Vechten Dielectric Classification of Crystal Structures Ionization Potentials and Band Structures Phys. Rev. Lett. 22 (14) (1969) pp K. S erberg et al. Crystal Structures and Phase Stability in Pseudobinary CaAl 2x Zn x J. Solid State Chem. 179 (8) (2006) pp D. Pettifor Bonding and Structure of Molecules and Solids (Oxford U.K.: Oxford University Press 1995). 7. C. Suh and K. Rajan Establishing Measurement Techniques for Mapping StructureProperty Relationships Mat. Sci. Tech. (accepted). 8. L. Eriksson et al. Multi and Megavariate Data Analysis Principles and Applications (Umeå Sweden: Umetrics Academy 1999). 9. R.A. Johnson and D.W. Wichern Applied Multivariate Statistical Analysis 5th Ed. (Upper Saddle River NY: Prentice Hall 2002). 10. K.E. Sickafus J.M. Wills and N.W. Grimes Structure of Spinel J. Am. Ceram. Soc. 82 (12) (1999) pp W.Y. Ching et al. Theoretical Prediction of the Structure and Properties of Cubic Spinel Nitrides J. Am. Ceram. Soc. 85 (1) (2002) pp Table A. Useful Descriptors for Spinel Nitrides and Relationships between Crystallographic Descriptors and Anion Parameter. All IDs Correspond to the Descriptors in Table I (from Reference 10) Crystallographic Analytical Descriptors Formulation (Number Linking Lattice Correspond Parameter with Anion to Those Cited Parameter (Taken from in Table I) Sickafus et al. 10 ) 3 3a(u 1/ 4) 4 a[2(u 3 / 8) (5 / 8 u) ] 20 ( 3 /8)a 21 (1/ 4)a 22 ( 2 /4)a 23 ( 11/8)a 24 ( 3 /4)a a(u 1/4) a(1/2 u) /2 2a{(u 3 / 8) 1/ 32} 28 3a(1/ 2 u) ANALYTICAL EXPRESSIONS FOR CRYSTAL CHEMISTRY: LINKING GEOMETRY TO BONDING As noted by R.M. Thompson and R.T. Down 24 crystal chemistry has traditionally considered the analysis of anioncation interactions as critical to the understanding of stability and a crystal structure s response to temperature pressure and composition. A pure hardsphere model of crystal geometry is not sufficient in addressing the link between the chemical identity of an atom and the geometry (coordination) of its environment as described by bond lengths and bond. There is a need to link the geometrical distortions associated with bonding relative to an ideal hard sphere model. Thompson and Down for instance have proposed formulations that account for the distortion in bond lengths and bond angles due to the iconicity of the bonding. This is quantified in terms of an anion parameter (u) that quantifies the distortion of the anion skeleton in a crystal by a measure of the a{2(u 1/ 4) (1/ 2 u) } a{(u 1/ 4) 2(1/ 2 u) } a{2(u 3 / 8) (u 1/ 8) } 3 3 (8 / 3)a (u 1/ 4) 3 3 (8 / 3)a (1/ 2 u) 3 (1/ 3)a (1/ 2 u)(u 1/ 4) 3 2 (16 / 3)a (1/ 2 u) (u 1/ 8) 3 2 (16 / 3)a (u 1/ 4) (5 / 8 u) 3 (1/ 192)a 12. P. Villars A ThreeDimensional Structure Stability Diagram for 998 Binary AB Intermetallic Compounds J. LessCommon Met. 92 (1983) pp J.K. Burdett G.D. Price and S.L. Price Factors Influencing SolidState Structure An Analysis Using Pseudopotential Radii Structural Maps Phys. Rev. B 24 (6) (1981) pp J.K. Burdett G.D. Price and S.L. Price Role of the CrystalField Theory in Determining the Structures of Spinels A. Am. Chem. Soc. 104 (1982) pp H. Haeuseler Structure Field Maps for Sulfides of Composition AB 2 X 4 J. Solid. State. Chem. 86 (1990) pp A. Zunger A Pseudopotential Viewpoint of the Electronic and Structural Properties of Crystals Structure and Bonding in Crystals Vol. I ed. M. O Keeffe and A. Navrotsky (New York: Academic average isotropic displacement of the anions from the ideal closestpacked structures. This distortion accounts for nearestneighbor interactions and the coordination of anions associated with different chemistries. Sickafus et al. 10 have developed analytical expressions linking lattice parameters and anion parameters specifically for spinel structures (see Table A). For the spinel geometry there are numerous bond lengths and bond angle distortions that need to be accounted for as anions in spinels usually are dilated away from their cubicclosepacked positions which in turn changes bond lengths bond angles interstice volumes and the symmetries of coordination polyhedra. To map all this information requires plotting the numerous relationships linking geometrical bond distortions to anion and lattice parameters. Some examples are given in Figure A. The discussion in the body of this paper takes the input variables associated with these equations tabulated in Table A and maps the high dimensional correlations between all these parameters using data dimensionality reduction techniques such as principal component analysis. From this the authors have developed predictive models using regression tools in this high dimensional space providing a datadriven approach to explore the multivariate nature of geometrybonding relationships in complex structures. 52 JOM January 2009
6 Press 1981) pp Y. Harada et al. New Crystal Structure Maps for Intermetallic Compounds J. Phys.: Condens. Matter 9 (1997) pp P. Villars and J.C. Phillips Quantum Structural Diagrams and HighTc Superconductivity Phys. Rev. B 37 (4) (1988) pp C. Suh and K. Rajan Virtual Screening and QSAR Formulations for Crystal Chemistry QSAR & Comb. Sci. 24 (1) (2005) pp R.J. Hill J.R. Craig and G.V. Gibbs Systematics of the Spinel Structure Type Phys. Chem. Miner. 4 (1979) pp R.D. Tobias An Introduction to Partial Least Squares Regression (Cary NC: SAS Institute Inc. 2007) 22. V. Kholodovych et al. Accurate Predictions of Cellular Response using QSPR: A Feasibility Test of Rational Design of Polymeric Biomaterials Polymer 45 (22) (2004) pp M.D. Segall et al. Population Analysis of Plane Wave Electronic Structure Calculations of Bulk Materials Phys. Rev. B 54 (23) (1996) pp R.M. Thompson and R.T. Downs Quantifying Distortion from Ideal ClosestPacking in a Crystal Structure with Analysis and Application Acta Crystallographica Section B 57 (2) (2001) pp Changwon Suh and Krishna Rajan are with the Department of Materials Science and Engineering Iowa State University Ames IA USA. Dr. Rajan can be reached at a b Figure A: (a) Bond angle as a function of anion parameter (b) polyhedral volume as a function of anion parameter. Vol. 61 No. 1 JOM 53
Ceramic Bonding. CaF 2 : large SiC: small
Recall ceramic bonding:  Mixed ionic and covalent.  % ionic character ( f ) increases with difference in electronegativity Large vs small ionic bond character: Ceramic Bonding CaF : large SiC: small
More informationCrystal Structure and Chemistry
Crystal Structure and Chemistry Controls on Crystal Structure Metallic bonding closest packing Covalent bonding depends on orbital overlap and geometry Ionic bonding Pauling s Rules Coordination Principle
More informationFACTOR ANALYSIS AND MULTIDIMENSIONAL SCALING
FACTOR ANALYSIS AND MULTIDIMENSIONAL SCALING Vishwanath Mantha Department for Electrical and Computer Engineering Mississippi State University, Mississippi State, MS 39762 mantha@isip.msstate.edu ABSTRACT
More informationPrincipal Component Analysis, A Powerful Scoring Technique
Principal Component Analysis, A Powerful Scoring Technique George C. J. Fernandez, University of Nevada  Reno, Reno NV 89557 ABSTRACT Data mining is a collection of analytical techniques to uncover new
More informationElectronegativity is a very useful concept for the explanation or understanding of chemical reactivity throughout the periodic table.
1.6. Review of Electronegativity (χ) CONCEPT: Electronegativity is a very useful concept for the explanation or understanding of chemical reactivity throughout the periodic table. There are many definitions
More informationAtomic Arrangement. Primer in Materials Spring
Atomic Arrangement Primer in Materials Spring 2017 30.4.2017 1 Levels of atomic arrangements No order In gases, for example the atoms have no order, they are randomly distributed filling the volume to
More informationFollowed by metals and inert gases  closepacked structures Deviations: BCC metals 'Ionic' compounds strive to follow the principles.
Reading: West 7 &8 Principles of Laves 1.Space Principle: Space is used most efficiently 2.Symmetry Principle: Highest possible symmetry is adopted 3.Connection Principle: There will be the most possible
More informationCHAPTER 4. Crystal Structure
CHAPTER 4 Crystal Structure We can assume minerals to be made of orderly packing of atoms or rather ions or molecules. Many mineral properties like symmetry, density etc are dependent on how the atoms
More informationStructural Characterization of Substituted Calcium Titanate Compounds Ca 1X La X Ti 1x Fe x O 3
Egypt. J. Solids, Vol. (27), No. (2), (2004) 213 Structural Characterization of Substituted Calcium Titanate Compounds Ca 1X La X Ti 1x Fe x O 3 A.M. Moustafa 1, I.S Ahmed Farag 1 and L.M. Salah 2 1
More informationModeling Mutagenicity Status of a Diverse Set of Chemical Compounds by Envelope Methods
Modeling Mutagenicity Status of a Diverse Set of Chemical Compounds by Envelope Methods Subho Majumdar School of Statistics, University of Minnesota Envelopes in Chemometrics August 4, 2014 1 / 23 Motivation
More informationBonding and Packing: building crystalline solids
Bonding and Packing: building crystalline solids The major forces of BONDING Gravitational forces: F = G m m 1 2 F = attractive forces between 2 bodies G = universal graviational constant (6.6767 * 10
More informationAP Chemistry A. Allan Chapter 8 Notes  Bonding: General Concepts
AP Chemistry A. Allan Chapter 8 Notes  Bonding: General Concepts 8.1 Types of Chemical Bonds A. Ionic Bonding 1. Electrons are transferred 2. Metals react with nonmetals 3. Ions paired have lower energy
More informationPredictive analysis on Multivariate, Time Series datasets using Shapelets
1 Predictive analysis on Multivariate, Time Series datasets using Shapelets Hemal Thakkar Department of Computer Science, Stanford University hemal@stanford.edu hemal.tt@gmail.com Abstract Multivariate,
More informationChem 241. Lecture 20. UMass Amherst Biochemistry... Teaching Initiative
Chem 241 Lecture 20 UMass Amherst Biochemistry... Teaching Initiative Announcement March 26 Second Exam Recap Ellingham Diagram Inorganic Solids Unit Cell Fractional Coordinates Packing... 2 Inorganic
More informationDATA ANALYTICS IN NANOMATERIALS DISCOVERY
DATA ANALYTICS IN NANOMATERIALS DISCOVERY Michael Fernandez OCEPostdoctoral Fellow September 2016 www.data61.csiro.au Materials Discovery Process Materials Genome Project Integrating computational methods
More informationAnalysis of a Large Structure/Biological Activity. Data Set Using Recursive Partitioning and. Simulated Annealing
Analysis of a Large Structure/Biological Activity Data Set Using Recursive Partitioning and Simulated Annealing Student: Ke Zhang MBMA Committee: Dr. Charles E. Smith (Chair) Dr. Jacqueline M. HughesOliver
More informationStructure and Dynamics : An Atomic View of Materials
Structure and Dynamics : An Atomic View of Materials MARTIN T. DOVE Department ofearth Sciences University of Cambridge OXFORD UNIVERSITY PRESS Contents 1 Introduction 1 1.1 Observations 1 1.1.1 Microscopic
More informationMetallic & Ionic Solids. Crystal Lattices. Properties of Solids. Network Solids. Types of Solids. Chapter 13 Solids. Chapter 13
1 Metallic & Ionic Solids Chapter 13 The Chemistry of Solids Jeffrey Mack California State University, Sacramento Crystal Lattices Properties of Solids Regular 3D arrangements of equivalent LATTICE POINTS
More informationCh. 9 NOTES ~ Chemical Bonding NOTE: Vocabulary terms are in boldface and underlined. Supporting details are in italics.
Ch. 9 NOTES ~ Chemical Bonding NOTE: Vocabulary terms are in boldface and underlined. Supporting details are in italics. I. Review: Comparison of ionic and molecular compounds Molecular compounds Ionic
More informationGeol /19/06 Labs 5 & 6 Crystal Chemistry Ionic Coordination and Mineral Structures
Geol 2311 9/19/0 Labs 5 & Crystal Chemistry Ionic Coordination and Mineral Structures Handout Oral Mineral Tray Report Samples Ionic Coordination Exercise Investigating Mineral Structures using XtalDraw
More informationF Orbitals and MetalLigand Bonding in Octahedral Complexes Ken Mousseau
F Orbitals and MetalLigand Bonding in Octahedral Complexes Ken Mousseau I. Abstract The independent study will compare metalligand bonding in octahedral complexes with rare lanthanide metals. A comparison
More informationKernel Density Topic Models: Visual Topics Without Visual Words
Kernel Density Topic Models: Visual Topics Without Visual Words Konstantinos Rematas K.U. Leuven ESATiMinds krematas@esat.kuleuven.be Mario Fritz Max Planck Institute for Informatics mfrtiz@mpiinf.mpg.de
More informationIonic Bonding. Example: Atomic Radius: Na (r = 0.192nm) Cl (r = 0.099nm) Ionic Radius : Na (r = 0.095nm) Cl (r = 0.181nm)
Ionic Bonding Ion: an atom or molecule that gains or loses electrons (acquires an electrical charge). Atoms form cations (+charge), when they lose electrons, or anions ( charge), when they gain electrons.
More informationApplication Note. The Optimization of Injection Molding Processes Using Design of Experiments
The Optimization of Injection Molding Processes Using Design of Experiments Problem Manufacturers have three primary goals: 1) produce goods that meet customer specifications; 2) improve process efficiency
More informationDiscriminative Direction for Kernel Classifiers
Discriminative Direction for Kernel Classifiers Polina Golland Artificial Intelligence Lab Massachusetts Institute of Technology Cambridge, MA 02139 polina@ai.mit.edu Abstract In many scientific and engineering
More informationThe effect of light impurities on the binding energy of hydrogen in magnesium metal and magnesium hydride
The effect of light impurities on the binding energy of hydrogen in magnesium metal and magnesium hydride Finnbogi Óskarsson Science Institute, University of Iceland, Dunhaga 3, IS107 Reykjavík, Iceland
More informationChapter 4: Bonding in Solids and Electronic Properties. Free electron theory
Chapter 4: Bonding in Solids and Electronic Properties Free electron theory Consider free electrons in a metal an electron gas. regards a metal as a box in which electrons are free to move. assumes nuclei
More informationSolids. properties & structure
Solids properties & structure Determining Crystal Structure crystalline solids have a very regular geometric arrangement of their particles the arrangement of the particles and distances between them is
More informationPhys 460 Describing and Classifying Crystal Lattices
Phys 460 Describing and Classifying Crystal Lattices What is a material? ^ crystalline Regular lattice of atoms Each atom has a positively charged nucleus surrounded by negative electrons Electrons are
More informationChapter 12: Structures & Properties of Ceramics
Chapter 12: Structures & Properties of Ceramics ISSUES TO ADDRESS... Structures of ceramic materials: How do they differ from those of metals? Point defects: How are they different from those in metals?
More informationAtomic Structure & Interatomic Bonding
Atomic Structure & Interatomic Bonding Chapter Outline Review of Atomic Structure Atomic Bonding Atomic Structure Atoms are the smallest structural units of all solids, liquids & gases. Atom: The smallest
More informationDimension Reduction and Classification Using PCA and Factor. Overview
Dimension Reduction and Classification Using PCA and  A Short Overview Laboratory for Interdisciplinary Statistical Analysis Department of Statistics Virginia Tech http://www.stat.vt.edu/consult/ March
More informationChapter 8. Bonding: General Concepts
Chapter 8 Bonding: General Concepts Chapter 8 Questions to Consider What is meant by the term chemical bond? Why do atoms bond with each other to form compounds? How do atoms bond with each other to form
More informationDefinitions, Closest packing schemes Interstitial sites Other packing schemes Polymorphism (disintegrating buttons) Alloys. Closest packing of coins
Definitions, Closest packing schemes Interstitial sites Other packing schemes Polymorphism (disintegrating buttons) Alloys Closest packing of coins AB closest packing of spheres ABC closest packing of
More informationneed another quantum number, m s it is found that atoms, substances with unpaired electrons have a magnetic moment, 2 s(s+1) where {s = m s }
M polyelectronic atoms need another quantum number, m s it is found that atoms, substances with unpaired electrons have a magnetic moment, 2 s(s+1) where {s = m s } Pauli Exclusion Principle no two electrons
More informationCHEM1902/ N2 November 2014
CHEM1902/4 2014N2 November 2014 The cubic form of boron nitride (borazon) is the secondhardest material after diamond and it crystallizes with the structure shown below. The large spheres represent
More informationDFT EXERCISES. FELIPE CERVANTES SODI January 2006
DFT EXERCISES FELIPE CERVANTES SODI January 2006 http://www.csanyi.net/wiki/space/dftexercises Dr. Gábor Csányi 1 Hydrogen atom Place a single H atom in the middle of a largish unit cell (start with a
More informationDrift Reduction For MetalOxide Sensor Arrays Using Canonical Correlation Regression And Partial Least Squares
Drift Reduction For MetalOxide Sensor Arrays Using Canonical Correlation Regression And Partial Least Squares R GutierrezOsuna Computer Science Department, Wright State University, Dayton, OH 45435,
More informationClass XI: Chemistry Chapter 4: Chemical Bonding and Molecular Structure Top Concepts
1 Class XI: Chemistry Chapter 4: Chemical Bonding and Molecular Structure Top Concepts 1. The attractive force which holds together the constituent particles (atoms, ions or molecules) in chemical species
More informationThe nature of special points on unit cell parameters temperature dependences for crystal substances
Z. Kristallogr. Suppl. 26 (2007) 447452 by Oldenbourg Wissenschaftsverlag, München 447 The nature of special points on unit cell parameters temperature dependences for crystal substances Stanislav K.
More informationSurface stress and relaxation in metals
J. Phys.: Condens. Matter 12 (2000) 5541 5550. Printed in the UK PII: S09538984(00)113864 Surface stress and relaxation in metals P M Marcus, Xianghong Qian and Wolfgang Hübner IBM Research Center, Yorktown
More informationCHAPTER 2. Atomic Structure And Bonding 21
CHAPTER 2 Atomic Structure And Bonding 21 Structure of Atoms ATOM Basic Unit of an Element Diameter : 10 10 m. Neutrally Charged Nucleus Diameter : 10 14 m Accounts for almost all mass Positive Charge
More informationLinear Models 1. Isfahan University of Technology Fall Semester, 2014
Linear Models 1 Isfahan University of Technology Fall Semester, 2014 References: [1] G. A. F., Seber and A. J. Lee (2003). Linear Regression Analysis (2nd ed.). Hoboken, NJ: Wiley. [2] A. C. Rencher and
More informationDiamond. There are four types of solid: Hard Structure  Tetrahedral atomic arrangement. What hybrid state do you think the carbon has?
Bonding in Solids Bonding in Solids There are four types of solid: 1. Molecular (formed from molecules)  usually soft with low melting points and poor conductivity. 2. Covalent network  very hard with
More informationCHAPTER3 CLASSIFICATION OF ELEMENTS AND PERIODICITY IN PROPERTIES OF ELEMENTS
CHAPTER3 CLASSIFICATION OF ELEMENTS AND PERIODICITY IN PROPERTIES OF ELEMENTS Mandeleev s Periodic Law: The properties of the elements are the periodic function of their atomic masses. Moseley, the English
More informationPart 1. Theory. SpaceGroup Symmetry and Atomic Displacements
Introduction to Isotropy Subgroups and Displacive Phase Transitions Harold T. Stokes and Dorian M. Hatch Brigham Young University, Provo, Utah April 2006 This is an introduction to the concepts of isotropy
More informationAsymmetry of Endofullerenes with Silver Atoms
Asymmetry of Endofullerenes with Silver Atoms V.S. Gurin PhysicoChemical Research Institute, Belarusian State University Leningradskaja str., 14, Minsk, 220080, BELARUS; Email: gurin@bsu.by; gurinvs@lycos.com
More informationCHEM 1364 Detailed Learning Outcomes Fall 2011 Buckley
CHEM 1364 Introduction: Matter and Measurement (Chapter 1) Textbook references to Brown, LeMay, Bursten, Murphy, and Woodward 12 th Edition Classification of matter Given sufficient information be able
More informationChemical Space: Modeling Exploration & Understanding
verview Chemical Space: Modeling Exploration & Understanding Rajarshi Guha School of Informatics Indiana University 16 th August, 2006 utline verview 1 verview 2 3 CDK R utline verview 1 verview 2 3 CDK
More informationSummation of Periodic Trends Factors Affecting Atomic Orbital Energies
Summation of Periodic Trends Factors Affecting Atomic Orbital Energies The Effect of Nuclear Charge (Z effective ) Higher nuclear charge lowers orbital energy (stabilizes the system) by increasing nucleuselectron
More informationFollowed by metals and inert gases  closepacked structures Deviations: BCC metals 'Ionic' compounds strive to follow the principles.
Reading: West 7 &8 Principles of Laves 1.Space Principle: Space is used most efficiently 2.Symmetry Principle: Highest possible symmetry is adopted 3.Connection Principle: There will be the most possible
More information1 A factor can be considered to be an underlying latent variable: (a) on which people differ. (b) that is explained by unknown variables
1 A factor can be considered to be an underlying latent variable: (a) on which people differ (b) that is explained by unknown variables (c) that cannot be defined (d) that is influenced by observed variables
More informationThe Nature of Laves Phases: An Explorative Investigation of the NbCo System
The Nature of Laves Phases: An Explorative Investigation of the NbCo System Daniel Grüner, Frank Stein 1, Martin Palm 1, Joachim Konrad 1, Tadahiro Yokosawa 2, Alim Ormeci, Walter Schnelle, Osamu Terasaki
More informationProperties of Liquids and Solids. Vaporization of Liquids. Vaporization of Liquids. Aims:
Properties of Liquids and Solids Petrucci, Harwood and Herring: Chapter 13 Aims: To use the ideas of intermolecular forces to: Explain the properties of liquids using intermolecular forces Understand the
More informationProperties of Liquids and Solids. Vaporization of Liquids
Properties of Liquids and Solids Petrucci, Harwood and Herring: Chapter 13 Aims: To use the ideas of intermolecular forces to: Explain the properties of liquids using intermolecular forces Understand the
More informationCovalent Bonding. In nature, only the noble gas elements exist as uncombined atoms. All other elements need to lose or gain electrons
In nature, only the noble gas elements exist as uncombined atoms. They are monatomic  consist of single atoms. All other elements need to lose or gain electrons To form ionic compounds Some elements share
More informationChapter 8. Bonding: General Concepts
Chapter 8 Bonding: General Concepts Chapter 8 Table of Contents 8.1 Types of Chemical Bonds 8.2 Electronegativity 8.3 Bond Polarity and Dipole Moments 8.4 Ions: Electron Configurations and Sizes 8.5 Energy
More informationRutile TiO 2 tetragonal unit cell with a = b = Å, c = Å Fig. 1.32a: Ti positions, 2 per cell, corner(0,0,0) and body center( 21
1 f) Rutile (TiO 2 ), cadmium iodide (CdI 2 ), cadmium chloride (CdCl 2 ) and caesium oxide (Cs 2 O) Together with fluorite, they represent the main AX 2 structure types. Rutile TiO 2 tetragonal unit cell
More informationCharge Analysis: Atoms in Molecules
Daubechies Wavelets in Electronic Structure Calculation: BigDFT Code Tutorial CECAM  GRENOBLE : Atoms in Molecules Ali Sadeghi Basel University 21 November 2011 An output of electronic structure calculations
More informationCoordination Chemistry: Bonding Theories. Crystal Field Theory. Chapter 20
Coordination Chemistry: Bonding Theories Crystal Field Theory Chapter 0 Review of the Previous Lecture 1. We discussed different types of isomerism in coordination chemistry Structural or constitutional
More informationPrincipal Component Analysis (PCA) Theory, Practice, and Examples
Principal Component Analysis (PCA) Theory, Practice, and Examples Data Reduction summarization of data with many (p) variables by a smaller set of (k) derived (synthetic, composite) variables. p k n A
More informationMonte Carlo Based Calculation of Electron Transport Properties in Bulk InAs, AlAs and InAlAs
Bulg. J. Phys. 37 (2010) 215 222 Monte Carlo Based Calculation of Electron Transport Properties in Bulk InAs, AlAs and InAlAs H. Arabshahi 1, S. Golafrooz 2 1 Department of Physics, Ferdowsi University
More informationPROBING THE (EMPIRICAL) QUANTUM STRUCTURE EMBEDDED IN THE PERIODIC TABLE WITH AN EFFECTIVE BOHR MODEL
Quim. Nova, Vol. 36, No. 2, 335339, 2013 PROBING THE (EMPIRICAL) QUANTUM STRUCTURE EMBEDDED IN THE PERIODIC TABLE WITH AN EFFECTIVE BOHR MODEL Wellington Nardin Favaro e Alejandro LópezCastillo* Departamento
More informationELECTRONIC STRUCTURE OF Pu 3+ AND Pu 4+ IMPURITY CENTERS IN ZIRCON INTRODUCTION
Journal of Structural Chemistry. Vol. 51, No. 1, pp. 18, 2010 Original Russian Text Copyright 2010 by M. V. Ryzhkov, A. L. Ivanovskii, A. V. Porotnikov, Yu. V. Shchapova, and S. L. Votyakov ELECTRONIC
More informationADVANCED CHEMISTRY CURRICULUM. Unit 1: Mathematical Representation in Chemistry
Chariho Regional School District  Science Curriculum September, 2016 ADVANCED CHEMISTRY CURRICULUM Unit 1: Mathematical Representation in Chemistry OVERVIEW Summary Measurements are fundamental to the
More informationModern Inorganic Chemistry (a)inorganic Materials
Modern Inorganic Chemistry (a)inorganic Materials (b)metal ions in Biology {built on principles established long long ago} Let us go through a small tour of some examples & current topics which make inorganic
More informationL11: Pattern recognition principles
L11: Pattern recognition principles Bayesian decision theory Statistical classifiers Dimensionality reduction Clustering This lecture is partly based on [Huang, Acero and Hon, 2001, ch. 4] Introduction
More informationIonic Bonding  Electrostatic Interactions and Polarization
Ionic Bonding  Electrostatic Interactions and Polarization Chemistry 754 Solid State Chemistry Dr. Patrick Woodward Lecture #13 BornHaber Cycle for NaCl It is energetically unfavorable for Na metal and
More informationCalculation of thermal expansion coefficient of Fe3Al with the addition of transition metal elements Abstract Introduction Methodology
Calculation of thermal expansion coefficient of Fe Al with the addition of transition metal elements Tatiana Seletskaia, Leonid Muratov, Bernard Cooper, West Virginia University, Physics Departement, Hodges
More informationMolecular Geometry. Dr. Williamson s Molecular Geometry Notes. VSEPR: Definition of Terms. Dr. V.M. Williamson Texas A & M University Student Version
Molecular Geometry Dr. V.M. Williamson Texas A & M University Student Version Valence Shell Electron Pair Repulsion VSEPR 1. Valence e to some extent 2. Electron pairs move as far away as possible to
More informationExploratory Factor Analysis and Principal Component Analysis
Exploratory Factor Analysis and Principal Component Analysis Today s Topics: What are EFA and PCA for? Planning a factor analytic study Analysis steps: Extraction methods How many factors Rotation and
More informationDIMENSION REDUCTION AND CLUSTER ANALYSIS
DIMENSION REDUCTION AND CLUSTER ANALYSIS EECS 833, 6 March 2006 Geoff Bohling Assistant Scientist Kansas Geological Survey geoff@kgs.ku.edu 8642093 Overheads and resources available at http://people.ku.edu/~gbohling/eecs833
More informationNomenclature 1 Monatomic Ions Answer Key
Nomenclature 1 Monatomic Ions Answer Key Free PDF ebook Download: Nomenclature 1 Monatomic Ions Answer Key Download or Read Online ebook nomenclature 1 monatomic ions answer key in PDF Format From The
More informationScale, structure and behaviour
Scale, structure and behaviour Lecture 2 MTX9100 Nanomaterjalid OUTLINE How are crystals structured? Why and how does nanoworld differ from the world we live in? When does size matter? What is the smallest
More informationbond energy energy required to break a chemical bond We can measure bond energy to determine strength of interaction
bond energy energy required to break a chemical bond We can measure bond energy to determine strength of interaction ionic compound a metal reacts with a nonmetal Ionic bonds form when an atom that
More informationSTRUCTURES OF MERCURY MERCAPTIDES
STRUCTURES OF MERCURY MERCAPTIDES PART 11. XRAY STRUCTURAL ANALYSIS OF MERCURY ETHYLMERCAPTIDE D. C. BRADLEY~ AND N. R. KUNCHUR~ Department of Chemistry, University of Western Ontario, London, Ontario
More informationThe solid state. Ga Ge As Se Br d 10 4s 2. Sn Xe 1.49 I Sb Te In d 10 5s 2. Pb 0.
Molecular shape The shapes of molecules: van t Hoff (1874): CH 4 tetrahedron Werner (1893): Pt(NH 3 ) 2 Cl 2 planar Lewis (1915): Electron pairs and octets Sidgwick and Powell (1940): Foundations of Valence
More informationChemistry 101 Chapter 9 CHEMICAL BONDING
CHEMICAL BONDING Chemical bonds are strong attractive force that exist between the atoms of a substance. Chemical bonds are commonly classified into 3 types: Ionic Bonding Ionic bonds form between metals
More informationPrincipal Component Analysis  PCA (also called KarhunenLoeve transformation)
Principal Component Analysis  PCA (also called KarhunenLoeve transformation) PCA transforms the original input space into a lower dimensional space, by constructing dimensions that are linear combinations
More informationENERGY BAND STRUCTURE OF ALUMINIUM BY THE AUGMENTED PLANE WAVE METHOD
ENERGY BAND STRUCTURE OF ALUMINIUM BY THE AUGMENTED PLANE WAVE METHOD L. SMR6KA Institute of Solid State Physics, Czeehosl. Acad. Sci., Prague*) The band structure of metallic aluminium has been calculated
More informationMultivariate Fundamentals: Rotation. Exploratory Factor Analysis
Multivariate Fundamentals: Rotation Exploratory Factor Analysis PCA Analysis A Review Precipitation Temperature Ecosystems PCA Analysis with Spatial Data Proportion of variance explained Comp.1 + Comp.2
More informationPrincipal Component Analysis and Singular Value Decomposition. Volker Tresp, Clemens Otte Summer 2014
Principal Component Analysis and Singular Value Decomposition Volker Tresp, Clemens Otte Summer 2014 1 Motivation So far we always argued for a highdimensional feature space Still, in some cases it makes
More informationCHEM J4 June 2013
CHEM110 013J4 June 013 Describe the periodic trends exhibited by atomic radii. Justify these trends in terms of principal quantum number, n, and effective nuclear charge, Z eff. Atomic radius decreases
More informationFactor Analysis (10/2/13)
STA561: Probabilistic machine learning Factor Analysis (10/2/13) Lecturer: Barbara Engelhardt Scribes: Li Zhu, Fan Li, Ni Guan Factor Analysis Factor analysis is related to the mixture models we have studied.
More informationGeneralized Linear Models (GLZ)
Generalized Linear Models (GLZ) Generalized Linear Models (GLZ) are an extension of the linear modeling process that allows models to be fit to data that follow probability distributions other than the
More informationCovalent Bonds Ch. Why do atoms bond? Atoms want noble gas configuration ( ) For bonds there is a transfer of electrons to get an octet of electrons
Covalent Bonds Ch. Why do atoms bond? Atoms want noble gas configuration ( ) For bonds there is a transfer of electrons to get an octet of electrons For covalent bonds there is a of electrons to get an
More informationMgAl 2 Ge 2 a new representative of the structure type CaAl 2 Si 2
Chem. Met. loys 5 (2012) 5965 Ivan Franko National University of Lviv www.chemetaljournal.org Mg 2 Ge 2 a new representative of the structure type Ca 2 2 Svitlana PUKAS 1 *, Liliya PYLYPCHAK 1, Oksana
More information10 th Grade Honors Chemistry
10 th Grade Honors Chemistry Scranton School District Scranton, PA 10 th Grade Honors Chemistry Prerequisite: Honors Biology, Geometry Be in compliance with the SSD Honors and AP Criteria Policy 10 th
More informationFor more info visit Chemical bond is the attractive force which holds various constituents together in a molecule.
Chemical bond: Chemical bond is the attractive force which holds various constituents together in a molecule. There are three types of chemical bonds: Ionic Bond, Covalent Bond, Coordinate Bond. Octet
More informationStructure and interactions in benzamide molecular crystals
Structure and interactions in benzamide molecular crystals Philipp Ectors 1, Dominique Ectors 2, Dirk Zahn 1 1) Lehrstuhl für Theoretische Chemie/ComputerChemieCentrum FriedrichAlexander Universität
More informationCHEMICAL BONDING. Chemical Bonds. Ionic Bonding. Lewis Symbols
CHEMICAL BONDING Chemical Bonds Lewis Symbols Octet Rule whenever possible, valence electrons in covalent compounds distribute so that each maingroup element is surrounded by 8 electrons (except hydrogen
More informationRegularized Discriminant Analysis and ReducedRank LDA
Regularized Discriminant Analysis and ReducedRank LDA Department of Statistics The Pennsylvania State University Email: jiali@stat.psu.edu Regularized Discriminant Analysis A compromise between LDA and
More informationFinal Overview. Introduction to ML. Marek Petrik 4/25/2017
Final Overview Introduction to ML Marek Petrik 4/25/2017 This Course: Introduction to Machine Learning Build a foundation for practice and research in ML Basic machine learning concepts: max likelihood,
More informationMelting of Li, K, Rb and Cs at high pressure
Melting of Li, K, Rb and Cs at high pressure R N Singh and S Arafin Abstract Lindemann s melting law has been used to develop analytical expression to determine the pressure (P) dependence of the melting
More informationThe Effect of Halogen Atom Substitution on Bond Angles in Halogenated Compounds
. Chemistry Internal Assessment The Effect of alogen Atom Substitution on s in alogenated Compounds Chemistry teacher support material 1 Research Question In this investigation I will look at whether the
More informationSTUDY ON CORROSION P HENOMENA OF STEELS IN PBBI FLOW
11 th International Conference on Nuclear Engineering Tokyo, JAPAN, April 3, 3 ICONE1136375 STUDY ON CORROSION P HENOMENA OF STEELS IN PBBI FLOW Yingxia Qi Research Laboratory for Nuclear Reactors Tokyo
More informationShapes of Molecules and Hybridization
Shapes of Molecules and Hybridization A. Molecular Geometry Lewis structures provide us with the number and types of bonds around a central atom, as well as any NB electron pairs. They do not tell us the
More informationAccounting for measurement uncertainties in industrial data analysis
Accounting for measurement uncertainties in industrial data analysis Marco S. Reis * ; Pedro M. Saraiva GEPSIPSE Group, Department of Chemical Engineering, University of Coimbra Pólo II Pinhal de Marrocos,
More informationBOND LENGTHS AND BOND ANGLES IN OCTAHEDRAL, TRIGONAL BIPYRAMIDAL, AND RELATED MOLECULES OF THE NONTRANSITION ELEMENTS'
BOND LENGTHS AND BOND ANGLES IN OCTAHEDRAL, TRIGONAL BIPYRAMIDAL, AND RELATED MOLECULES OF THE NONTRANSITION ELEMENTS' ABSTRACT The stereochemistry of molecules in which there are five or six pairs of
More information7. Variable extraction and dimensionality reduction
7. Variable extraction and dimensionality reduction The goal of the variable selection in the preceding chapter was to find least useful variables so that it would be possible to reduce the dimensionality
More information